DOI: 10.1038/ncomms14081

OPEN

Disorder enabled band structure engineering of a topological insulator surface Yishuai Xu1, Janet Chiu1, Lin Miao1,2, Haowei He1, Zhanybek Alpichshev3,4, A. Kapitulnik4, Rudro R. Biswas5 & L. Andrew Wray1,6

Three-dimensional topological insulators are bulk insulators with Z2 topological electronic order that gives rise to conducting light-like surface states. These surface electrons are exceptionally resistant to localization by non-magnetic disorder, and have been adopted as the basis for a wide range of proposals to achieve new quasiparticle species and device functionality. Recent studies have yielded a surprise by showing that in spite of resisting localization, topological insulator surface electrons can be reshaped by defects into distinctive resonance states. Here we use numerical simulations and scanning tunnelling microscopy data to show that these resonance states have signiﬁcance well beyond the localized regime usually associated with impurity bands. At native densities in the model Bi2X3 (X ¼ Bi, Te) compounds, defect resonance states are predicted to generate a new quantum basis for an emergent electron gas that supports diffusive electrical transport.

1 Department of Physics, New York University, New York, New York 10003, USA. 2 Advanced Light Source, Lawrence Berkeley National Laboratory, Berkeley, California 94720, USA. 3 Massachusetts Institute of Technology, Department of Physics, Cambridge, Massachusetts 02139, USA. 4 Department of Physics, Stanford University, Stanford, California 94305, USA. 5 Department of Physics and Astronomy, Purdue University, West Lafayette, Indiana 47907, USA. 6 NYU-ECNU Institute of Physics at NYU Shanghai, 3663 Zhongshan Road North, Shanghai 200062, China. Correspondence and requests for materials should be addressed to R.R.B. (email: [email protected]) or to L.A.W. (email: [email protected]).

NATURE COMMUNICATIONS | 8:14081 | DOI: 10.1038/ncomms14081 | www.nature.com/naturecommunications

1

ARTICLE

2

a

Resonance

Non-resonant Hig h

(nm )

40

10 – 50 meV

30

200 – 400 meV

DO S

20

10

0

0

0

b

10

20

30

40 0 a axis (nm)

10

20

30

40

4 Total DOS (arb. units)

hree-dimensional topological insulators (TI) with the chemical formula M2X3 (M ¼ Bi, Sb; X ¼ Se, Te) are characterized by a single-Dirac-cone surface state1–3, and have been widely investigated as model materials for TI surface physics. Shortly after the discovery of the ﬁrst TI’s, it was established that standard effects of defect disorder such as backscattering and localization are greatly suppressed in TI surface states4–11. Altogether with the intuition that topological properties of band structure should be inherently impervious to weak perturbations, this led to a pervasive characterization that topological interfaces are essentially blind to the presence of non-magnetic defects. It is only with the recent advent of more detailed non-perturbative numerical investigations and targeted scanning tunnelling microscopy (STM) experiments12–25 that elements of this picture have been overturned. It is now known that, rather than being blind to defects, topological Dirac cone electrons actually bind loosely to atomic point defects in energy levels that fall very close to the Dirac point (see states labelled ‘resonance’ in Fig. 1b), and can radically redeﬁne electronic structure relevant to the Dirac transport regime. In isotropic Dirac models of TI surface states, strongly perturbing non-magnetic defects are theoretically expected to create circular s-wave resonance states, such as those plotted in Fig. 1a. Experimentally, these states have been observed in STM measurements of density of states (DOS) immediately above the Dirac point of topological insulator Bi2Se3 (see Fig. 1a (left) inset patch). Three bright spots in the STM image represent coherent interference with a slight t1% admixture of f-wave symmetry (Supplementary Note 2) because of anisotropy not considered in the accompanying simulation. The combined impact of multiple randomly distributed defects on the electronic structure has not yet been evaluated, and is the subject of the present work. Theoretical treatments of lattice defects are usually carried out in the single impurity approximation, since multiple impurities do not lead to emergent coherent bandstructures. Large modiﬁcations to the band structure of non-TI materials are only achieved through heterostructure growth or fractional alloying. The ‘impurity bands’ associated with electrons on minority impurity sites are generally disregarded as being non-ideal for electronic transport. These bands exhibit miniscule dispersions, and strong defect potentials or reduced dimensionality cause the electronic states to be Anderson localized26,27 over relevant device lengthscales. A typical example is the well-studied manganese impurity band in Ga1 xMnxAs, whose dispersion across the Brillouin zone is far smaller than its intrinsic width along the energy axis, meaning that the electrons are effectively localized to isolated lattice sites28,29. In the following, in contrast, we ﬁnd that uncompensated lattice defects at low densities (ro0.1%) in non-amorphous TIs provide a mechanism for band structure engineering that is not shared in a conventional semiconducting system. Theoretically, it is expected that Anderson localization will be forbidden on the TI surface with non-magnetic impurities30–34 and backscattering is suppressed relative to forward scattering4,5,9, leading to greater itinerancy for impurity-derived band structure. Moreover, the electronic density of states falls to zero at a surface Dirac point, making it possible for defect resonance states to dominate the absolute density of states. In the following discussions we will show that these conditions enable new defectderived electronic dispersions, providing viable channels for diffusive electrical transport. We also ﬁnd that these emergent electronic band structures can superﬁcially appear to be gapped, and resemble Dirac point anomalies that have been seen by angle resolved photoemission spectroscopy (ARPES) in

ba x is

T

NATURE COMMUNICATIONS | DOI: 10.1038/ncomms14081

t

No 2

an

Resonance

3

on

s -re

n

n-

No

re

so

na

D0

nt

1

0 –0.2

–0.1

0 0.1 Energy (eV)

0.2

0.3

Figure 1 | Defects on a TI surface. (a) A simulation of density of states (DOS) in different energy regions at a TI surface with 100 100 lattice sites and six randomly placed point defects (density r ¼ 0.06%). One of the simulated defect resonance states has been overlaid with a three-fold symmetrized STM density of states image obtained 70 meV above the Dirac point of Bi2Se3. (b) The Dirac point energy (D0) and resonance state peak are labelled on the energy-resolved DOS distribution for a large 350 350 site surface with r ¼ 0.06% defect density. Red shading indicates states in which electrons adhere closely to defects.

TI compounds that have no known time reversal symmetry broken ground state35–38. Results Defect resonance states of Dirac electrons. We will focus on defect resonance states in the popular Bi2Se3 xTex family of single-Dirac-cone TIs1–3, so as to make quantitative comparisons to STM measurements. However, our results are applicable to other TI surface states with isolated Dirac cones. In this material family, structural point defects tend to occur with a density of rt0.1% per formula unit, and have been found to overlap with the surface state in the outermost quintuple layer of the lattice15,39 (see Supplementary Note 1). Intensive characterization of Bi2Se3 has found that the density and type-range of defects can be tuned over a broad range by adjusting sample growth conditions39. For Se-poor and stoichiometric synthesis, defects near a cleaved surface are predominantly selenium vacancies positioned in the centre of the outermost quintuple layer of the lattice. Interstitial atoms and replacement defects can be common at the surface of Se-rich or quench-cooled samples. The chemical potential can be shifted as a separate parameter via methods that include bulk doping, surface dosing, and electrostatic gating40–43. Defect resonance states have been observed by STM less than 200 meV above the surface Dirac point, surrounding point defects14,15 and at step edges between plateaus differing in height by one quintuple layer18,19. Characteristic local density of states (LDOS) distributions measured by STM at the defect

NATURE COMMUNICATIONS | 8:14081 | DOI: 10.1038/ncomms14081 | www.nature.com/naturecommunications

ARTICLE

NATURE COMMUNICATIONS | DOI: 10.1038/ncomms14081

b

–22.5 eV –45 eV –90 eV

c

–22.5 eV –45 eV –90 eV Exp.

2 eV 3.8 eV 5 eV Exp.

7 6 5 4

2

3 2

1

LDOS (arb. units)

a

3

DOS (arb. units)

Step defect

Point defect

4

1 0 –300

0 –100

100

300 0

50

Energy (meV) 0.20

100

150

0

100

200

300

Energy relative to D0 (meV) High

e

d

f

0.15

Intensity

Energy (eV)

0.10 0.05 0 −0.05

U = –22.5 eV

U = –45 eV

U = –90 eV

= 0.06%

= 0.06%

= 0.06%

−0.10 −0.15

0 0

0.02

0.04

0

0.02

0.04

0

0.02

0.04

0.06

Momentum Kr (Å–1)

Figure 2 | The non-magnetic defect potential. (a) The DOS distribution for point defects with r ¼ 0.06% density at different defect potentials. (b,c) The local DOS distribution of point (r ¼ 0.06%) and step defect resonance states at different ‘U’ defect potentials. Black experimental curves are reproduced from STM investigations in refs 15,18. (d–f) The ARPES spectral function of a large TI surface with randomly distributed point defects is modelled as a function of defect potential.

lattice sites are plotted as black curves in Fig. 2b,c. Theoretical analyses of isolated local impurities have shown that these resonance states arise naturally when strong scalar potentials are introduced to a surface occupied by spin-helical TI Dirac cone electrons12,13,15–17. For an isolated defect described as a point potential with amplitude U, the resonance state is split from the Dirac point by an energy roughly proportional to U 1. In the following, we numerically approach the problem of multiple impurity scattering on the surface states of TIs with a single Dirac cone, which is otherwise theoretically intractable. We use a basis of spinor plane waves44 on a discrete hexagonal real-space lattice, with lattice parameter a ¼ 4.2 Å corresponding to Bi2Se3 xTex surface atomic spacings. We have used the impurity-free spin-helical Hamiltonian, Hk ¼ v0(k s), with Dirac velocity v0 ¼ 3.0 eV Å chosen to be intermediate between Bi2Se3 and Bi2Te3. When a large surface with a typical rB0.06% defect density is modelled in this way, we ﬁnd that B2 electronic states per defect are added near the Dirac point (see Supplementary Note 1; Supplementary Fig. 4), resulting in a new DOS peak that becomes increasingly visible as the defect potential grows (Fig. 2a). Isolating the LDOS at defect cores on Bi2Se3 reveals that a defect potential of U ¼ 45 eV accurately reproduces the resonance state energy and LDOS line shape obtained in STM studies, which is plotted in Fig. 2b. The very different experimental line shape of a step edge defect can likewise be reproduced by considering the tunnelling barrier generated with a repulsive potential of U ¼ 3.8 eV applied to each atom along the step edge path (Fig. 2c). These comparisons are evidence that our numerical approach is able to quantitatively capture the physics observed in experiments.

New delocalized electronic structure. The resonance states associated with this defect distribution reveal a novel structure in the momentum-resolved electron annihilation (ARPES) spectral function, modelled in Fig. 2d–f. The resonance itself shows up as a discontinuity in the ARPES spectral function. As the defect potential strength increases, the surface Dirac point (termed D0), as well as the discontinuity associated with the resonance state LDOS maximum (ER) move down in energy (Fig. 3h). When the defect potential crosses a critical value of UtB45 eV, a new local maximum appears in the spectrum at point), roughly 50 meV above the D0 Dirac point, and K ¼ 0 (G will henceforth be referred to as ‘D1’. As the defect resonance state converges on E ¼ 0 eV with increasing potential strength, the region between D0 and D1 begins to qualitatively resemble a band gap, as has been seen at the Dirac point of TI crystals with non-magnetic defects in refs 35,36. Unlike a true band gap, which is theoretically disallowed6, the momentum-integrated total DOS distribution contains a local maximum within the seemingly gapped region (Fig. 2a). A remarkable evolution of the electronic structure also occurs when the defect density is increased (see Fig. 3a–c series). When the defect density is tripled to r ¼ 0.18%, the faint local maximum D1 becomes the dispersion minimum of an upper band that is clearly disconnected from the D0 Dirac cone. The D0 upper Dirac cone maintains its dispersion for small momenta Kt0.02 Å, out to more than 50 meV from the Dirac point, and becomes dispersionless at larger momenta, as would be expected for a more typical impurity band. For all of these impurity densities, the upper D0 Dirac cone dispersion is signiﬁcantly larger than the energy axis intrinsic width, which is dEB0.02 and 0.04 eV at half maximum intensity in Fig. 3b,c, respectively.

NATURE COMMUNICATIONS | 8:14081 | DOI: 10.1038/ncomms14081 | www.nature.com/naturecommunications

3

ARTICLE 0.25

NATURE COMMUNICATIONS | DOI: 10.1038/ncomms14081

a

0.20

Fermi Velocity × 4/5

b

Fermi Velocity × 1/2

c

d

Fermi Velocity × 1/8

Fermi Velocity × 1/40

High

0.10

D1

E*

0.05 0

U = –45 eV = 0.02%

−0.05

U = –45 eV = 0.06%

Intensity

Energy (eV)

0.15

Zeeman field = 0.18%

U = –45 eV = 0.18%

D0

−0.10 0 −0.15 0

0.04

0.08

0

0.04

0.08

0

0.04

0.08

0

0.04

0.08

Momentum Kr (Å–1)

e

f

15 nm

E*

0.06

D1

E* 0.04

ER ER

D1

0

D0

–25 0

0.05 0.1 0.15 0.2 0 Defect density (%)

0 –0.02

D0

g

0.02

Energy (eV)

25 D0 min (meV)

0.08

= 0.06%

U = –45 eV

h

–0.04

–50 –100 –150 Defect Pot. U (eV)

Figure 3 | Emergent band structure. (a–c) The momentum resolved spectral function of a large TI surface with randomly distributed point defects is shown as a function of defect density ‘r’. Arrows indicate radial axis twist velocity vy(E, K). The critical energy E*, resonance energy ER and K ¼ 0 local maxima (D0 and D1) are labelled on panel c. (d) The non-magnetic twist velocity simulation in panel c is repeated for equivalently strong magnetic defects (J ¼ 45 eV). (e,f) The spatial distribution of the LDOS minimum associated with the Dirac point is shown (e) from STM measurements on Se-poor Bi2Se3 d and (f) from a simulation for U ¼ 45, with black dots representing the locations of electron donating Se vacancy defects. Both distributions can be well represented in the same ±25 meV range. (g,h) The Dirac points, resonance state LDOS maximum, and critical energy E* are plotted as a function of defect density and defect potential. The image in panel (e) is adapted with permission from ref. 39, copyrighted by the American Physical Society.

Higher defect densities are also associated with further lowering of the D0 Dirac point energy. An STM map obtained on a Se vacancy-rich Bi2Se3 d surface shows that spatial ﬂuctuations in the energy of the D0 LDOS minimum are highly correlated with defect density (Fig. 3e). Simulating the observed Se vacancies with a U ¼ 45 defect potential reproduces the qualitative spatial distribution of the D0 LDOS minimum (Fig. 3f). These modelling results can be plotted in the same ±25 meV range as the STM data, showing that the energy scale of ﬂuctuations is accurately captured, even though ﬁne details may be inconsistent because of missing information about defects outside of the STM map, or deeper in the crystal. We note that the spatial distribution of defects observed by STM is very uniform and uncorrelated, and is not readily distinguished from the random defect conﬁgurations used in our simulations (see Poisson distribution overlay in Supplementary Fig. 1). The emergence of new spectral features at high defect density is closely related to the fraction of states near the Dirac point that can be attributed as defect resonance states. In the absence of defects, the total number states within an energy E of pﬃﬃ 2 of a NE2 the Dirac point is NE ¼ 34pv 2 , where N is the total number 0 of 2D surface lattice sites. Setting NE equal to the approximate number of q resonance states (NE ¼ NR2rN) gives a new energy ﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ 8pv02 r ? ﬃﬃ p scale, E ¼ 2 , which we ﬁnd to have a novel physical 3a

signiﬁcance. As can be see in Fig. 3g,h, we ﬁnd that a local maximum associated with the emergent D1 feature becomes 4

visible when the resonance state energy ER becomes smaller than E*. These simulations also reveal that the resonance energy may be tuned not only by changing the impurity strength, as has been theoretically predicted before, but also by increasing the impurity concentration, a fact that is technologically signiﬁcant because the impurity strength is usually not tunable. With the experimentally ﬁtted defect potential U ¼ 45 eV, the resonance energy crosses E* when the defect density becomes larger than r ¼ 0.02%, resulting in the easily visible emergent features in Fig. 3b,c. To evaluate the ability of the emergent coherent impurity band-like features to carry mobile charge, we have calculated the twist velocity, vy, for conﬁgurations with 300 300 sites (300 sites ¼ 126 nm per side). These are shown in Fig. 3a–c, as vectors overlaid at local maxima of the modelled ARPES spectrum. The twist velocity of a quantum state is proportional to the magnitude of a persistent DC current carried by that state in the presence of an electric ﬁeld (see Methods), and in the scattering-free limit is equivalent to the group velocity of the electronic band. It is calculated as the gradient of the state energies with respect to a phase twist around the system boundary. We ﬁnd that the twist velocities of band features at energies E40 eV have similar amplitudes, and are approximately proportional to the apparent slope in momentum space, suggesting that all of these features are viable bands for charge transport. However, twist velocities decay towards zero as the upper D0 Dirac cone disperses into the seemingly gapped region

NATURE COMMUNICATIONS | 8:14081 | DOI: 10.1038/ncomms14081 | www.nature.com/naturecommunications

ARTICLE

NATURE COMMUNICATIONS | DOI: 10.1038/ncomms14081

b

Frequency

c

High

0.15

V / VD

Log (Participation ratio)

Log (Participation ratio)

V / VD

V@KΓM= 0.05 Å−1

System length (L/sites)

3

J=45 eV =0.18%

10

40

0 50 0

10–3

0

5

10–5

−3 .

5 −4 .

−5

−0.15

−4

J=45 eV =0.06%

= 0.02% = 0.06% = 0.18% 1/N

0

−0.05

10–4

20

0

10–2

0

0.05

Non-res band Res band Fitted curve

J=45 eV

10

Participation ratio

0.1

−0.1

f 10–3

30

Magnetic

Energy (eV)

System length (L/sites)

e

0.15

U=−45 eV =0.18% 2

System length (L/sites)

50

d

10−2

10

5

50

10

−3 .

.5 −4

−5

−0.15

–5

2

U=−45 eV =0.06%

= 0.02% = 0.06% = 0.18% 1/N

10

−0.1

10–4

10−1

30 0 40 0 50 0

−0.05

Non-res band Res band Fitted curve V@KΓM= 0.05 Å−1

U=–45 eV

20 0

Participation ratio

0

−4

Energy (eV)

res=0.057%

0.05

10–3

10 0

Non-magnetic 0.1

3

0

10

a

System length (L/sites)

Figure 4 | Real-space structure. (a) A histogram of energy-resolved participation ratio for a 350 350 site simulated surface with r ¼ 0.06% density scalar defects. The resonance region is circled, and labelled with the density of resonance states contained within the circle. (b) The dependence of resonance state participation ratios on the edge-length L in an L L simulation is plotted for different defect densities. (c) The dependence of twist velocity along a linear L 100 system at momentum K ¼ 0.05 Å 1 is shown for the resonance band and upper non-resonance band. The dashed ﬁt curve is proportional to L 0.91. Panels d–f show the same quantities for magnetic defects, using a ﬁt curve proportional to L 1.33 for f.

beneath the D1 feature, particularly at momenta of k\0.05 Å, and this may greatly limit carrier mobility for certain values of the chemical potential (see evaluation of twist and band velocities in Supplementary Note 1; Supplementary Figs 2 and 3). Velocities are relatively large in the lower D0 Dirac cone, where states are energetically distant from the resonance states, and maximal velocities are found immediately beneath D0, where elastic scattering is minimal because of the vanishing density of states near a 2D Dirac point. For comparison, a similar simulation with magnetic defects instead of a U ¼ 45 eV scalar ﬁeld is shown in Fig. 3d, representing a case in which the topological protection against Anderson localization is expected to fail45. We have approximated each magnetic defect by a localized J ¼ 45 eV exchange ﬁeld perfectly aligned with the þ z-axis, perpendicular to the surface (see Methods). In this magnetic scenario, even though disorder of the magnetic moment vectors has been neglected, twist velocities are still reduced by an additional order of magnitude near the Dirac point because of Anderson localization. We have also investigated the transport characteristics of the potential disorder-induced band structure by an alternate metric, the participation ratios of the quantum eigenstates. The participation ratio46,47 of an electronic wavefunction is the sum of squares of the site-resolved probability densities (see Methods). For itinerant electronic states that can participate in electronic transport, it decays as the inverse of the total number of sites in the system (N 1), for large system sizes. On the other hand, for localized states, the participation ratio converges on a non-zero value as system size increases beyond the localization length of the wavefunction. The participation ratios of the

energy eigenstates in the presence of scalar and magnetic disorder are compared in Fig. 4. We ﬁnd that in the latter case, Anderson localized states around the resonances display large participation ratios that saturate with system size (Fig. 4e), while topological protection against localization ensures that the participation ratios for the comparable scalar potential disorder case vary inversely as the system size, for large system sizes (Fig. 4b). Calculating the twist velocities for larger system sizes shows a similar trend (Fig. 4c,f), in which scalar defect potentials allow diffusive transport (vy\L 1), being topologically protected against Anderson localization, unlike conventional impurity bands, represented here by the same surface states in the presence of magnetic disorder of comparable strength. Discussion Impurity-induced carrier control is the cornerstone of the semiconductor industry, and band structure engineering via disorder is the natural successor of such disorder-induced functionalization of electronic materials. In conventional 2D materials, Anderson localization prevents impurity bands from acting as viable carriers for diffusive charge transport. In this work, we have shown that this restriction is ameliorated in the surface states of topological insulators, in the presence of moderate potential disorder that does not break time reversal symmetry. Using numerical techniques veriﬁed by comparison to experimental observations, we have demonstrated that a new impurity band structure emerges in the TI surface states in the presence of scalar potential disorder, and that these states remain diffusive and are able to participate in transport processes. We have contrasted this novel behaviour, when topological

NATURE COMMUNICATIONS | 8:14081 | DOI: 10.1038/ncomms14081 | www.nature.com/naturecommunications

5

ARTICLE

NATURE COMMUNICATIONS | DOI: 10.1038/ncomms14081

protection against localization is present, to the more conventional situation when magnetic disorder of comparable strength is present, when Anderson localization prevents diffusive transport in the impurity band. Our results also shed light on some less understood DOS anomalies on TI surface states that have been reported in the literature. ARPES experiments have previously resolved gap-like features35–37 and Dirac point elongation38 in the spectrum of TI surface states, in the absence of any timereversal breaking effects. The experiment in ref. 37 presents a particularly telling case. In this work, incident photon polarization was tuned to eliminate the dominant evensymmetry photoemission channel from Bi2Se3 along the high M axis. Defect resonance states do not have spatial symmetry G reﬂection symmetry because of their random distribution, and would not be intrinsically suppressed by this symmetry factor. This defect-sensitive measurement geometry revealed a gap-like dispersion, with the upper Dirac cone bands appearing to converge more than E450 meV above the Dirac point, as expected from our calculations for the D1 feature. We have shown that these observations may be attributed to the effects discussed above, arising from scalar potential disorder alone. The emergent band structure associated with defects is very narrowly separated from nearby bands in momentum, and will be difﬁcult to cleanly resolve in ARPES experiments. The energy-axis widths of bands in our calculations are 2–3 times narrower than those actually observed in Bi2Se3, indicating that factors not considered here such as phonon scattering and surface inhomogeneity may play a signiﬁcant role in the low energy physics, and may obscure the role of defectderived states. Nonetheless, the existence of defect resonance states immediately above the Dirac point of these compounds is well known from STM measurements, and the new physics discussed in this work are direct consequences of the interplay between these resonance states and other established elements of TI surface physics. The numerical evaluations of electron mobility and localization discussed above show that the emergent band structure identiﬁed in these simulations is viable as a basis for conductivity, and that band structure engineering is possible via non-magnetic defects in a TI system, driven by unique factors such as the lack of Anderson localization and the vanishing of DOS near a 2D Dirac point. Methods Energetics and state basis at the TI surface. STM data and LDOS curves were obtained by the procedures described in refs 15,18. The surface state is modelled as a spin-helical 2D Dirac cone occupying a discrete hexagonal real-space lattice with repeating boundary conditions, and is essentially a discretized version of the model in refs 13,15. The kinetic Hamiltonian is given by Hk ¼ v0(k s), with velocity v0 ¼ 3.0 eV chosen to be intermediate between Bi2Se3 and Bi2Te3. The real space basis includes two spin-degenerate states per lattice site. The kinetic Hamiltonian is diagonalized on this basis, and the resulting momentum-space basis is reduced by applying a high energy cutoff W ¼ 0.4 eV to exclude high energy states that would not conform to a Dirac dispersion. Defects are createdPby perturbing sites at selected coordinates i with a scalar energy term. as Hd ¼ i Uni , where ni is the number operator, and the full Hamiltonian H ¼ Hk þ Hd is diagonalized. The convention of creating point defects as triangular three-site clusters with a perturbation strength of U/3 on each site is adopted to give three-fold rotational symmetry, as seen experimentally14,15, though calculated spectra do not strongly differentiate between differently sized small site clusters (Supplementary Fig. 6). The Hamiltonian is numerically diagonalized, and the ARPES spectral function is deﬁned as the energy- and momentum-resolved spectral function of single particle annihilation, convoluted by a 10 meV half-width Lorentzian: I ðE; kÞ¼

X h f jak;s jai2 f ;a;s

5 meV=p ðE EðaÞÞ2 þ ð5 meVÞ2

This represents the spectral function for photoemission with the z-axis photon polarization, which acts with even reﬂection symmetry and removes 6

ð1Þ

electrons from the dominant pz orbital component of the Bi2Se3 xTex surface state. Energy-momentum dispersions were found to be rotationally isotropic, and have been rotationally averaged to obtain a small spacing between states on the momentum axis. Figures in the paper use the rotationally averaged ‘radial’ momentum (Kr), and single-axis spectral functions can be found in Supplementary Fig. 5. For smaller system sizes considered in Fig. 4, it was necessary to average over several randomly generated defect conﬁgurations to achieve convergence of the twist velocity and participation ratio. Additional modelling details are found in Supplementary Note 3. Metrics of localization. Adding a phase twist y at the system boundary provides an easy way to identify the degree to which electronic states are localized. This is achieved by the standard method of shifting the momentum (K-space) basis of the Hilbert space by an offset of Ky ¼yx =Lx k^x þ yy =Ly k^y , where Lx (Ly) is the width of the system along the x (y ) axis. A velocity termed the ‘twist velocity’ can be calculated for individual eigenstates |ai as vy(a) ¼ rKyEa (using numerical derivatives), and represents the velocity of a persistent current. The energy- and momentum-resolved twist velocity (vy(E, k)) displayed on ARPES spectral intensity maxima in Fig. 3 is calculated via a weighted average of states within ±10 meV of the energy E, as: P vy ðaÞjhk; sjaij2 a;s v y ðE; kÞ ¼ P ð2Þ jhk; sjaij2 a;s

Here, hk; sj represents the free particle eigenstates that have momentum k. When divided by the width of the system L along the indicated axis, the phase twist has units of wave number. The numerical derivative is performed at a p small but nonzero twist value of y¼ 10 along the k^ direction to break degeneracies and avoid possible ﬁnite size nesting effects. The participation ratio is deﬁned as: X Pa ¼ n2i;a ; ð3Þ i

where the sum is over all sites in the system, and ni,a is the LDOS on site i of |ai, which is an eigenstate of the full Hamiltonian. Data availability. The data and source code that support the ﬁndings of this study are available from the corresponding authors on reasonable request.

References 1. Zhang, H. et al. Topological insulators in Bi2Se3, Bi2Te3 and Sb2Te3 with a single Dirac cone on the surface. Nat. Phys. 5, 438–442 (2009). 2. Xia, Y. et al. Observation of a large-gap topological-insulator class with a single Dirac cone on the surface. Nat. Phys. 5, 398–402 (2009). 3. Chen, Y. L. et al. Experimental realization of a three-dimensional topological insulator, Bi2Te3. Science 325, 178–181 (2009). 4. Hasan, M. Z. & Kane, C. L. Colloquium: topological insulators. Rev. Mod. Phys. 82, 3045 (2010). 5. Qi, X.-L. & Zhang, S.-C. Topological insulators and superconductors. Rev. Mod. Phys. 83, 1057 (2011). 6. Fu, L., Kane, C. L. & Mele, E. J. Topological insulators in three dimensions. Phys. Rev. Lett. 98, 106803 (2007). 7. Hsieh, D. et al. Observation of unconventional quantum spin textures in topological insulators. Science 323, 919–922 (2009). 8. Moore, J. E. & Balents, L. Topological invariants of time-reversal-invariant band structures. Phys. Rev. B 75, 121306 (2007). 9. Roushan, P. et al. Topological surface states protected from backscattering by chiral spin texture. Nature 460, 1106–1109 (2009). 10. Alpichshev, Z. et al. STM imaging of electronic waves on the surface of Bi2Te3: topologically protected surface states and hexagonal warping effects. Phys. Rev. Lett. 104, 016401 (2010). 11. Qi, X.-L., Hughes, T. L. & Zhang, S.-C. Topological ﬁeld theory of time-reversal invariant insulators. Phys. Rev. B 78, 195424 (2008). 12. Black-Schaffer, A. M. & Yudin, D. Spontaneous gap generation on the surface of weakly interacting topological insulators using nonmagnetic impurities. Phys. Rev. B 90, 161413 (2014). 13. Biswas, R. R. & Balatsky, A. V. Impurity-induced states on the surface of threedimensional topological insulators. Phys. Rev. B 81, 233405 (2010). 14. Teague, M. L. et al. Observation of Fermi-energy dependent unitary impurity resonances in a strong topological insulator Bi2Se3 with scanning tunneling spectroscopy. Solid State Commun. 152, 747–751 (2012). 15. Alpichshev, Z. et al. STM Imaging of Impurity Resonances on Bi2Se3. Phys. Rev. Lett. 108, 206402 (2012). 16. Black-Schaffer, A. M. & Balatsky, A. V. Subsurface impurities and vacancies in a three-dimensional topological insulator. Phys. Rev. B 86, 115433 (2012). 17. Black-Schaffer, A. M. & Balatsky, A. V. Strong potential impurities on the surface of a topological insulator. Phys. Rev. B 85, 121103 (2012).

NATURE COMMUNICATIONS | 8:14081 | DOI: 10.1038/ncomms14081 | www.nature.com/naturecommunications

ARTICLE

NATURE COMMUNICATIONS | DOI: 10.1038/ncomms14081

18. Alpichshev, Z., Analytis, J. G., Chu, J.-H., Fisher, I. R. & Kapitulnik, A. STM imaging of a bound state along a step on the surface of the topological insulator Bi2Te3. Phys. Rev. B 84, 041104 (2011). 19. Dmitriev, A. Yu., Fedotov, N. I., Nasretdinova, V. F. & Zaitsev-Zotov, S. V. Effect of surface defects and few-atomic steps on the local density of states of the atomically-clean surface of Bi2Se3 topological insulator. JETP Lett. 100, 398–402 (2014). 20. Wang, J. et al. Power-law decay of standing waves on the surface of topological insulators. Phys. Rev. B 84, 235447 (2011). 21. Biswas, R. R. & Balatsky, A. V. Scattering from surface step edges in strong topological insulators. Phys. Rev. B 83, 075439 (2011). 22. Rizzo, B., Arrachea, L. & Moskalets, M. Transport phenomena in helical edge state interferometers: a Green’s function approach. Phys. Rev. B 88, 155433 (2013). 23. Fu, Z. G., Zhang, P., Wang, Z. & Li, S. S. Quantum corrals and quantum mirages on the surface of a topological insulator. Phys. Rev. B 84, 235438 (2011). 24. Fu, Z. G. et al. Anisotropic Fabry-Prot resonant states conﬁned within nanosteps on the topological insulator surface. Sci. Rep. 4, 5544 (2014). 25. Liu, Q., Qi, X.-L. & Zhang, S.-C. Stationary phase approximation approach to the quasiparticle interference on the surface of a strong topological insulator. Phys. Rev. B 85, 125314 (2012). 26. Anderson, P. W. Absence of diffusion in certain random lattices. Phys. Rev 109, 1492–1505 (1958). 27. Abrahams, E., Anderson, P. W., Licciardello, D. C. & Ramakrishnan, T. V. Scaling theory of localization: absence of quantum diffusion in two dimensions. Phys. Rev. Lett. 42, 673–676 (1979). 28. Ernst, A., Sandratskii, L. M., Bouhassoune, M., Henk, J. & Lu¨ders, M. Weakly dispersive band near the fermi level of GaMnAs due to Mn interstitials. Phys. Rev. Lett. 95, 237207 (2005). 29. Okabayashi, J. et al. Angle-resolved photoemission study of Ga1 xMnxAs. Phys. Rev. B 64, 125304 (2001). 30. Konig, E. J., Ostrovsky, P. M., Protopopov, I. V. & Mirlin, A. D. Metal-insulator transition in two-dimensional random fermion systems of chiral symmetry classes. Phys. Rev. B 85, 195130 (2012). 31. Fu, L. & Kane, C. L. Topology, delocalization via average symmetry and the symplectic anderson transition. Phys. Rev. Lett. 109, 246605 (2012). 32. Ostrovsky, P. M., Gornyi, I. V. & Mirlin, A. D. Interaction-induced criticality in Z2 topological insulators. Phys. Rev. Lett. 105, 036803 (2010). 33. Ostrovsky, P. M., Gornyi, I. V. & Mirlin, A. D. Quantum criticality and minimal conductivity in graphene with long-range disorder. Phys. Rev. Lett. 98, 256801 (2007). 34. Ryu, S., Mudry, C., Obuse, H. & Furusaki, A. Z2 topological term, the global anomaly, and the two-dimensional symplectic symmetry class of anderson localization. Phys. Rev. Lett. 99, 116601 (2007). 35. Xu, S.-Y. et al. Hedgehog spin texture and Berry’s phase tuning in a magnetic topological insulator. Nat. Phys. 8, 616–622 (2012). 36. Xu, S.-Y. et al.Dirac point spectral weight suppression and surface ‘gaps’ in nonmagnetic and magnetic topological insulators. Preprint at http://arxiv.org/ abs/1206.0278v3 (2012). 37. Jozwiak, C. et al. Photoelectron spin-ﬂipping and texture manipulation in a topological insulator. Nat. Phys. 9, 293–298 (2013). 38. Miao, L. et al. Quasiparticle dynamics in reshaped helical Dirac cone of topological insulators. Proc. Natl Acad. Sci. 110, 2758–2762 (2013). 39. Dai, J.-X. et al. Toward the intrinsic limit of the topological insulator Bi2Se3. Phys. Rev. Lett. 117, 106401 (2016).

40. Hsieh, D. et al. A tunable topological insulator in the spin helical Dirac transport regime. Nature 460, 1101–1105 (2009). 41. Checkelsky, J. G., Ye, J., Onose, Y., Iwasa, Y. & Tokura, Y. Dirac-fermionmediated ferromagnetism in a topological insulator. Nat. Phys. 8, 729–733 (2012). 42. Wray, L. A. et al. Observation of topological order in a superconducting doped topological insulator. Nat. Phys. 6, 855859 (2010). 43. Wray, L. A. et al. A topological insulator surface under strong Coulomb, magnetic and disorder perturbations. Nat. Phys. 7, 32–37 (2011). 44. Nomura, K., Koshino, M. & Ryu, S. Topological delocalization of twodimensional massless dirac fermions. Phys. Rev. Lett. 99, 146806 (2007). 45. Sessi, P. et al. Dual nature of magnetic dopants and competing trends in topological insulators. Nat. Commun. 7, 12027 (2016). 46. Bell, R. J. & Dean, P. Atomic vibrations in vitreous silica. Disc. Faraday Soc. 50, 55–61 (1970). 47. Thouless, D. J. Electrons in disordered systems and the theory of localization. Phys. Rep. 13C, 93–142 (1974).

Acknowledgements We are grateful for discussions with W. Wu, P. Hohenberg and Y.-D. Chuang. Work at Stanford University was supported by the Department of Energy Grant DE-AC02-76SF00515. R.R.B. was supported by Purdue University startup funds.

Authors contributions Y.X. and J.C. carried out the numerical modelling with assistance from H.H. and guidance from R.R.B. and L.A.W.; Y.X., J.C., L.M., R.R.B. and L.A.W. participated in the analysis, ﬁgure planning and draft preparation; Z.A. and A.K. performed and analysed the STM experiments; L.A.W. was responsible for the conception and the overall direction, planning and integration among different research units.

Additional information Supplementary Information accompanies this paper at http://www.nature.com/ naturecommunications Competing ﬁnancial interests: The authors declare no competing ﬁnancial interests. Reprints and permission information is available online at http://npg.nature.com/ reprintsandpermissions/ How to cite this article: Xu, Y. et al. Disorder enabled band structure engineering of a topological insulator surface. Nat. Commun. 8, 14081 doi: 10.1038/ncomms14081 (2017). Publisher’s note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional afﬁliations. This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/

r The Author(s) 2017

NATURE COMMUNICATIONS | 8:14081 | DOI: 10.1038/ncomms14081 | www.nature.com/naturecommunications

7